### Transcription

Thermodynamics and Phase DiagramsArthur D. PeltonCentre de Recherche en Calcul Thermodynamique(CRCT)École Polytechnique de MontréalC.P. 6079, succursale Centre-villeMontréal QC Canada H3C 3A7Tél :1-514-340-4711 (ext. 4531)Fax :1-514-340-5840E-mail : [email protected](revised Aug. 10, 2011)

2

1IntroductionAn understanding of phase diagrams is fundamental and essential to the study ofmaterials science, and an understanding of thermodynamics is fundamental to anunderstanding of phase diagrams. A knowledge of the equilibrium state of a systemunder a given set of conditions is the starting point in the description of manyphenomena and processes.A phase diagram is a graphical representation of the values of the thermodynamicvariables when equilibrium is established among the phases of a system. Materialsscientists are most familiar with phase diagrams which involve temperature, T, andcomposition as variables.Examples are T-composition phase diagrams for binarysystems such as Fig. 1 for the Fe-Mo system, isothermal phase diagram sections ofternary systems such as Fig. 2 for the Zn-Mg-Al system, and isoplethal (constantcomposition) sections of ternary and higher-order systems such as Fig. 3a and Fig. 4.However, many useful phase diagrams can be drawn which involve variables otherthan T and composition. The diagram in Fig. 5 shows the phases present at equilibriumin the Fe-Ni-O2 system at 1200oC as the equilibrium oxygen partial pressure (i.e.chemical potential) is varied. The x-axis of this diagram is the overall molar metal ratioin the system. The phase diagram in Fig. 6 shows the equilibrium phases present whenan equimolar Fe-Cr alloy is equilibrated at 925oC with a gas phase of varying O2 and S2partial pressures.For systems at high pressure, P-T phase diagrams such as thediagram for the one-component Al2SiO5 system in Fig. 7a show the fields of stability ofthe various allotropes. When the pressure in Fig. 7a is replaced by the volume of thesystem as y-axis, the “corresponding” V-T phase diagram of Fig. 7b results.enthalpy of the system can also be a variable in a phase diagram.TheIn the phasediagram in Fig. 3b, the y-axis of Fig. 3a has been replaced by the molar enthalpydifference (hT – h25) between the system at 25oC and a temperature T. This is the heatwhich must be supplied or removed to heat or cool the system adiabatically between25oC and T.The phase diagrams in Figs. 1-7 are only a small sampling of the many possibletypes of phase diagram sections. These diagrams and several other useful types ofphase diagrams will be discussed in this chapter. Although these diagrams appear to3

have very different geometries, it will be shown that actually they all obey exactly thesame geometrical rules.The theme of this chapter is the relationship between phase diagrams andthermodynamics.To understand phase diagrams properly it has always beennecessary to understand their thermodynamic basis.However, in recent years therelationship between thermodynamics and phase diagrams has taken on a new andimportant practical dimension. With the development of large evaluated databases ofthe thermodynamic properties of thousands of compound and solutions, and of softwareto calculate the conditions for chemical equilibrium (by minimizing the Gibbs energy), itis possible to rapidly calculate and plot desired phase diagram sections ofmulticomponent systems.Most of the phase diagrams shown in this chapter werecalculated thermodynamically with the FactSage software and databases (seeFactSage in the list of websites at the end of this chapter).Several large integrated thermodynamic database computing systems have beendeveloped in recent years (See list of websites at the end of this chapter.). Thedatabases of these systems have been prepared by the following procedure. For everycompound and solution phase of a system, an appropriate model is first developedgiving the thermodynamic properties as functions of T, P and composition. Next, allavailable thermodynamic and phase equilibrium data from the literature for the entiresystem are simultaneously optimized to obtain one set of critically-evaluated, selfconsistent parameters of the models for all phases in 2-component, 3-component and, ifdata are available, higher-order subsystems. Finally, the models are used to estimatethe properties of multicomponent solutions from the databases of parameters of thelower-order subsystems.The Gibbs-energy minimization software then accesses thedatabases and, for given sets of conditions (T, P, composition.) calculates thecompositions and amounts of all phases at equilibrium. By calculating the equilibriumstate as T, composition, P, etc. are varied systematically, the software generates thephase diagram. As mentioned above, although the phase diagram sections shown inFigs. 1-7 are seemingly quite different topologically, they actually obey the same simplerules of construction and hence can all be calculated by the same algorithm.Sec. 2 provides a review of the fundamentals of thermodynamics as required for4

the interpretation and calculation of phase diagrams of all types. In Sec. 3 the GibbsPhase Rule is developed in a general form suitable for the understanding of phasediagrams involving a wide range of variables including chemical potentials, enthalpy,volume, etc.Sec. 4 begins with a review of the thermodynamics of solutions andcontinues with a discussion of the thermodynamic origin of binary T-composition phasediagrams, presented in the classical manner involving common tangents to curves ofGibbs energy. A thorough discussion of all features of T-composition phase diagramsof binary systems is presented in Sec. 5, with particular stress on the relationshipbetween the phase diagram and the thermodynamic properties of the phases. A similardiscussion of T-composition phase diagrams of ternary systems is given in Sec. 6.Isothermal and isoplethal sections as well as polythermal projections are discussed.Readers conversant in binary and ternary T-composition diagrams may wish toskip Secs. 4, 5 & 6 and pass directly to Sec. 7 where the geometry of general phasediagram sections is developed.In this section are presented: the general rules ofconstruction of phase diagram sections; the proper choice of axis variables andconstants required to give a single-valued phase diagram section with each point of thediagram representing a unique equilibrium state; and a general algorithm for calculatingall such phase diagram sections.Sec. 8 outlines the techniques used to develop large thermodynamic databasesthrough evaluation and modeling. Sec. 9 treats the calculation of equilibrium and nonequilibrium cooling paths of multicomponent systems.In Sec. 10, order/disordertransitions and their representation on phase diagrams are discussed.2ThermodynamicsThis section is intended to provide a review of the fundamentals ofthermodynamics as required for the interpretation and calculation of phase diagrams.The development of the thermodynamics of phase diagrams will be continued insucceeding sections.2.1The First and Second Laws of ThermodynamicsIf the thermodynamic system under consideration is permitted to exchange both5

energy and mass with its surroundings, the system is said to be open. If energy but notmass may be exchanged, the system is said to be closed. The state of a system isdefined by intensive properties, such as temperature and pressure, which areindependent of the mass of the system, and by extensive properties, such as volumeand internal energy, which vary directly as the mass of the system.2.1.1NomenclatureExtensive thermodynamic properties will be represented by upper case symbols.For example, G Gibbs energy in J. Molar properties will be represented by lower casesymbols. For example, g G/n molar Gibbs energy in J mol-1 where n is the totalnumber of moles in the system.2.1.2The First LawThe internal energy of a system, U, is the total thermal and chemical bond energystored in the system. It is an extensive state property.Consider a closed system undergoing a change of state which involves anexchange of heat, dQ, and work, dW, with its surroundings. Since energy must beconserved:dU n dQ dW(1)This is the First Law. The convention is adopted whereby energy passing from thesurroundings to the system is positive. The subscript on dUn indicates that the systemis closed (constant number of moles.)It must be stressed that dQ and dW are not changes in state properties. For asystem passing from a given initial state to a given final state, dUn is independent of theprocess path since it is the change of a state property; however dQ and dW are, ingeneral, path-dependent.2.1.3The Second LawFor a rigorous and complete development of the Second Law, the reader isreferred to standard texts on thermodynamics. The entropy of a system, S, is an6

extensive state property which is given by Boltzmann’s equation as:S kB ln t(2)where kB is Boltzmann’s constant and t is the multiplicity of the system. Somewhatloosely, t is the number of possible equivalent microstates in a macrostate, that is thenumber of quantum states for the system which are accessible under the applicableconditions of energy, volume, etc. For example, for a system which can be describedby a set of single-particle energy levels, t is the number of ways of distributing theparticles over the energy levels, keeping the total internal energy constant. At lowtemperatures, most of the particles will be in or near the ground state. Hence, t and Swill be small. As the temperature, and hence U, increase, more energy levels becomeoccupied. Consequently t and S increase. For solutions, an additional contribution to tarises from the number of different possible ways of distributing the atoms or moleculesover the lattice or quasilattice sites. (See Sec 4.1.5). Again somewhat loosely, S can besaid to be a measure of the disorder of a system.During any spontaneous process, the total entropy of the universe will increase forthe simple reason that disorder is more probable than order.That is, for anyspontaneous process:dStotal ( dS dSsurr ) 0(3)where dS and dSsurr are the entropy changes of the system and surroundingsrespectively. The existence of a state property S which satisfies Eq. (3) is the essenceof the Second Law.Eq. (3) is a necessary condition for a process to occur. However, even if Eq. (3) issatisfied the process may not actually be observed if there are kinetic barriers to itsoccurrence. That is, the Second Law says nothing about the rate of a process whichcan vary from extremely rapid to infinitely slow.It should be noted that the entropy change of the system, dS, can be negative fora spontaneous process as long as the sum (dS dSsurr) is positive. For example,during the solidification of a liquid, the entropy change of the system is negative in7

going from the liquid to the more ordered solid state. Nevertheless, a liquid below itsmelting point will freeze spontaneously because the entropy change of the surroundingsis sufficiently positive due to the transfer of heat from the system to the surroundings. Itshould also be stressed that in passing from a given initial state to a given final state,the entropy change of the system dS is independent of the process path since it is thechange of a state property. However, dSsurr is path-dependent.2.1.4The Fundamental Equation of ThermodynamicsConsider an open system at equilibrium with its surroundings and at internalequilibrium. That is, no spontaneous irreversible processes are taking place. Supposethat a change of state occurs in which S, V (volume) and ni (number of moles ofcomponent i in the system) change by dS, dV and dni.Such a change of stateoccurring at equilibrium is called a reversible process, and the corresponding heat andwork terms are dQrev and dWrev. We may then write:where:dU ( U S )v,n dS ( U V )s,n dV μ idni(4)μ i ( U ni )s,v, nj i(5)μi is the chemical potential of component i which will be discussed in Sec. 2.7.The absolute temperature is given as:T ( U S )v,n(6)We expect that temperature should be defined such that heat flows spontaneously fromhigh to low T. To show that T as given by Eq. (6) is, in fact, such a thermal potential,consider two closed systems, isolated from their surroundings but in thermal contactwith each other, exchanging only heat at constant volume. Let the temperatures of thesystems be T1 and T2 and let T1 T2.Suppose that heat flows from system 1 tosystem 2. Then dU2 - dU1 0. Therefore, from Eq. (6):dS dS1 dS2 dU1 / T1 dU2 / T2 08(7)

That is, the flow of heat from high to low temperature results in an increase in totalentropy and hence, from the Second Law, is spontaneous.The second term in Eq. (4) is clearly (-PdV), the work of reversible expansion.From Eq. (6) the first term in Eq. (4) is equal to TdS, and this is then the reversible heat:(8)T dS dQ revThat is, in the particular case of a process which occurs reversibly, (dQrev/T) is pathindependent since it is equal to the change of a state property dS. Eq. (8) is actuallythe definition of entropy in the classical development of the Second Law.Eq. (4) may now be written as:dU T dS - P dV μidni(9)Eq. (9), which results from combining the First and Second Laws is called thefundamental equation of thermodynamics. We have assumed that the only work term isthe reversible work of expansion (sometimes called “PV work”.) In general, in thischapter, this will be the case.If other types of work occur, then non-PV terms,dWrev(non-PV), must be added to Eq. (9). For example, if the process is occurring in agalvanic cell, then dWrev(non-PV) is the reversible electrical work in the external circuit.Eq. (9) can thus be written more generally as:dU T dS P dV μ i dni dWrev(non PV )2.2(10)EnthalpyEnthalpy, H, is an extensive state property defined as:H U PV(11)Consider a closed system undergoing a change of state which may involve irreversibleprocesses (such as chemical reactions.)Although the overall process may beirreversible, we shall assume that any work of expansion is approximately reversible(that is, the external and internal pressures are equal) and that there is no work other9

than work of expansion. Then, from Eq. (1):dUn dQ - P dV(12)From Eqs (11) and (12) it follows that:dH n dQ V dP(13)Furthermore, if the pressure remains constant throughout the process, then:dHp dQ p(14)Integrating both sides of Eq. (14) gives:ΔHp Qp(15)That is, the enthalpy change of a closed system in passing from an initial to a final stateat constant pressure is equal to the heat exchanged with the surroundings. Hence, for aprocess occurring at constant pressure the heat is path-independent since it is equal tothe change of a state property. This is an important result. As an example, supposethat the intitial state of a system consists of 1.0 mol of C and 1.0 mol of O2 at 298.15 Kat 1.0 bar pressure and the final state is one mole of CO2 at the same temperature andpressure. The enthalpy change of this reaction is:C O 2 CO 2ΔHo298.15 393.52 kJ(16)(where the superscript on ΔHo298 .15 indicates the “standard state” reaction involvingpure solid graphite, CO2 and O2 at 1.0 bar pressure.) Hence, an exothermic heat of- 393.52 kJ will be observed, independent of the reaction path, provided only that thepressure remain constant throughout the process. For instance, during the combustionreaction the reactants and products may attain high and unknown temperatures.However, once the CO2 product has cooled back to 298.15 K, the total heat which hasbeen exchanged with the surroundings will be -393.52 kJ independent of theintermediate temperatures.In Fig. 8 is shown the standard molar enthalpy of Fe as a function of temperature.10

()oThe y-axis, hTo h298.15 , is the heat required to heat one mole of Fe from 298.15 K toa temperature T at constant pressure. The slope of the curve is the molar heat capacityat constant pressure:c p ( dh dT ) P(17)From Eq. (17) we obtain the following expression for the heat required to heat one moleof a substance from a temperature T1 to a temperature T2 at constant P (assuming nophase changes in the interval):(hT2T2) c hT1 pdT(18)T1The enthalpy curve can be measured by the technique of drop calorimetry, or the heatcapacity can be measured directly by adiabatic calorimetry.The standard equilibrium temperature of fusion (melting) of Fe is 1811 K as shownon Fig. 8. The fusion reaction is a first-order phase change since it occurs at constanttemperature. The standard molar enthalpy of fusion Δhfo is 13.807 kJ mol-1 as shownon Fig. 8. It can also be seen on Fig. 8 that Fe undergoes two other first-order phasechanges, the first from α (bcc) to γ (fcc) Fe at Tαo γ 1184.8 K and the second from γto δ (bcc) at 1667.5 K. The enthalpy changes are, respectively, 1.013 and 0.826 kJmol-1. The Curie temperature, Tcurie 1045 K, which is also shown on Fig. 8, will bediscussed in Sec. 10.2.3Gibbs EnergyThe Gibbs energy (also called the Gibbs free energy, or simply the free energy),G, is defined as:G H – TS(19)As in Sec. 2.2, we consider a closed system and assume that the only work term is thework of expansion and that this is reversible. From Eqs (13) and (19):11

dGn dQ V dP – T dS – S dT(20)Consequently, for a process occurring at constant T and P in a closed system:dGT,P,n dQP – T dS dHP – T dS(21)Consider the case where the “surroundings” are simply a heat reservoir at atemperature equal to the temperature T of the system.That is, no irreversibleprocesses occur in the surroundings which receive only a reversible transfer of heat(-dQ) at constant temperature. Therefore, from Eq. (8):dSsurr - dQ/T(22)Substituting into Eq. (21) and using Eq. (3) yields:dGT,P,n - T dSsurr – T dS - T dStotal 0(23)Eq. (23) may be considered to be a special form of the Second Law for a processoccurring in a closed system at constant T and P. From Eq. (23) such a process will bespontaneous if dG is negative.For our purposes in this chapter Eq. (23) is the most useful form of the SecondLaw.An objection might be raised that Eq. (23) applies only when the surroundings areat the same temperature T as the system.However, if the surroundings are at adifferent temperature, we simply postulate a hypothetical heat reservoir which is at thesame temperature as the system, and which lies between the system and surroundings,and we consider the irreversible transfer of heat between the reservoir and the realsurroundings as a second separate process.Substituting Eqs (8) and (22) into Eq. (23) gives:dGT,P,n (dQ – dQrev) 0(24)In Eq. (24), dQ is the heat of the actual process, while dQrev is the heat which would beobserved were the process occurring reversibly. If the actual process is reversible, thatis if the system is at equilibrium, then dQ dQrev and dG 0.12

As an example, consider the fusion of Fe in Fig. 8. At Tfo 1181 K, solid andliquid are in equilibrium. That is, at this temperature melting is a reversible process.Therefore, at 1811 K:dgof dhof Tdsof 0(25)Therefore the molar entropy of fusion at 1811 K is given by:(Δsof Δ hof T)when T Tfo(26)Eq. (26) applies only at the equilibrium melting point. At temperatures below and abovethis temperature the liquid and solid are not in equilibrium. Above the melting point,Δg fo 0 and melting is a spontaneous process (liquid more stable than solid). Belowthe melting point, Δg fo 0 and the reverse process (solidification) is spontaneous. Asthe temperature deviates progressively further from the equilibrium melting point themagnitude of Δg fo , that is of the driving force, increases.We shall return to thissubject in Sec. 4.2.2.4Chemical EquilibriumConsider first the question of whether silica fibers in an aluminum matrix at 500 Cwill react to form mullite, Al6Si2O13 :13 SiO 6 Al 9 Si Al Si O26 2 1322(27)If the reaction proceeds with the formation of dξ moles of mullite then, from thestoichiometry of the reaction, dnSi (9/2) dξ , dnAl -6 dξ , and dnSiO2 -13/2 dξ . Sincethe four substances are essentially immiscible at 500 C, their Gibbs energies are equalto their standard molar Gibbs energies, g io (also known as the standard chemicalpotentials μio as defined in Sec. 2.7), the standard state of a solid or liquid compoundbeing the pure compound at P 1.0 bar. The Gibbs energy of the system then varies13

as:oodG dξ goAl6Si2O13 92 gSi 132 gSiO 6goAl ΔGo 830kJ2(28)where ΔGo is called the standard Gibbs energy change of reaction (27) at 500 C.Since ΔG 0, the formation of mullite entails a decrease in G. Hence, the reaction willproceed spontaneously so as to minimize G. Equilibrium will never be attained and thereaction will proceed to completion.2.4.1Equilibria Involving a Gaseous PhaseAn ideal gas mixture is one which obeys the ideal gas equation of state:PV nRT(29)where n is the total number of moles. Further, the partial pressure of each gaseousspecies in the mixture is given by:piV niRT(30)where n Σni and P Σpi (Dalton’s Law for ideal gases). R is the ideal gas constant.The standard state of a gaseous compound is the pure compound at a pressure of 1.0bar. It can easily be shown that the partial molar Gibbs energy gi (also called thechemical potential μi as defined in Sec. 2.7) of a species in an ideal gas mixture is givenoin terms of its standard molar Gibbs energy, g i (also called the standard chemicalopotential μi ) by:gi gio RT ln pi(31)The final term in Eq. (31) is entropic. As a gas expands at constant temperature itsentropy increases.Consider a gaseous mixture of H2, S2 and H2S with partial pressures pH2 pS2 andpH2S. The gases can react according to2H2 S2 2H2S(32)If reaction (32) proceeds to the right with the formation of 2dξ moles of H2S, then the14

Gibbs energy of the system varies as:dG dξ 2gH2S 2gH2 gS2( 2gHo 2 S 2gHo 2 gSo 2() RT 2lnpH2S 2lnpH2 lnpS2( ΔGo RT ln pH2 2S pH 22 pS 12))(33) ΔGΔG, which is the Gibbs energy change of reaction (32), is thus a function of the partialpressures. If ΔG 0, then the reaction will proceed to the right so as to minimize G. In aclosed system, as the reaction continues with the production of H2S, pH2S will increasewhile pH2 and pS2 will decrease. As a result, ΔG will become progressively less negative.Eventually an equilibrium state will be reached when dG/dξ ΔG 0.For the equilibrium state, therefore:ΔGo RT ln K( RT ln pH2 2S pH 22 pS 12)(34)equilibriumwhere K, the "equilibrium constant" of the reaction, is the one unique value of the ratio(p)2p 2 p 1 for which the system will be in equilibrium at the temperature T.H 2S H 2 S 2If the initial partial pressures are such thatΔG 0, then reaction (32) will proceed tothe left in order to minimize G until the equilibrium condition of Eq. (34) is attained.As a further example, consider the possible precipitation of graphite from agaseous mixture of CO and CO2. The reaction is:2CO C CO2Proceeding as above, we can write:15(35)

dG dξ gC gCO2 2 gCO(() 2o goC gCO2 2goCO RT ln pCO2 pCO( 2 ΔGo RT ln pCO2 pCO)( 2 ΔG RT lnK RT ln pCO2 pCO()(36))) 2If pCO2 pCOis less than the equilibrium constant K, then precipitation of graphite willoccur in order to decrease G.Real situations are, of course, generally more complex. To treat the deposition ofsolid Si from a vapour of SiI4, for example, we must consider the formation of gaseousI2, I and SiI2 so that three independent reaction equations must be written:SiI4(g) Si(sol) 2I2(g)(37)SiI4(g) SiI2(g) I2(g)(38)I2(g) 2I(g)(39)The equilibrium state, however, is still that which minimizes the total Gibbs energy of thesystem. This is equivalent to satisfying simultaneously the equilibrium constants ofreactions (37) to (39).Equilibria involving reactants and products which are solid or liquid solutions willbe discussed in Sec. 4.1.4.2.4.2Predominance DiagramsPredominance diagrams are a particularly simple type of phase diagram whichhave many applications in the fields of hot corrosion, chemical vapor deposition, etc.Furthermore, their construction clearly illustrates the principles of Gibbs energyminimization.A predominance diagram for the Cu-SO2-O2 system at 700oC is shown in Fig. 9.The axes are the logarithms of the partial pressures of SO2 and O2 in the gas phase.The diagram is divided into areas or domains of stability of the various solid compoundsof Cu, S and O. For example, at point Z, where pSO2 10 2 and pO2 10 7 bar, thestable phase is Cu2O. The conditions for coexistence of two and three solid phases are16

indicated respectively by the lines and triple points on the diagram. For example, alongthe line separating the Cu2O and CuSO4 domains the equilibrium constant 3 2 2K pSOpOof the following reaction is satisfied:22Cu2O 2SO2 3/2 O2 2CuSO4(40)log K ΔG o RT 2 log pSO2 3 / 2 log pO2 constant(41)Hence, along this line:This line is thus straight with slope (-3/2)/2 - 3/4.We can construct Fig. 9 following the procedure of Bale et al. (1986). We formulatea reaction for the formation of each solid phase, always from one mole of Cu, andinvolving the gaseous species whose pressures are used as the axes (SO2 and O2 inthis example):Cu 21 O2 CuOΔG ΔGo RT ln pO 1/22(42)Cu 41 O2 21 Cu2OΔG ΔGo RTln pO 1/42(43)Cu SO2 CuS O2Cu SO2 O2 CuSO 4()(44)()(45) 1ΔG ΔGo RT ln pO2 pSO2 1ΔG ΔGo RT ln pSOp 12 O2and similarly for the formation of Cu2S, Cu2SO4 and Cu2SO5.The values of ΔGo are obtained from tables of thermodynamic properties. For anygiven values of pSO2 and pO2 , ΔG for each formation reaction can then be calculated. Thestable compound is simply the one with the most negative ΔG. If all the ΔG values arepositive, then pure Cu is the stable compound.By reformulating Eqs. (42) to (45) in terms of, for example, S2 and O2 rather thanSO2 and O2, a predominance diagram with log pS2 and log pO2 as axes can be constructed. Logarithms of ratios or products of partial pressures can also be used as axes.Along the curve shown by the crosses on Fig. 9 the total pressure is 1.0 bar. Thatis, the gas consists not only of SO2 and O2, but of other species such as S2 whose17

equilibrium partial pressures can be calculated. Above this line the total pressure isgreater than 1.0 bar even though the sum of the partial pressures of SO2 and O2 may beless than 1.0 bar.A similar phase diagram of RT ln pO2 versus T for the Cu-O2 system is shown inFig. 10. For the formation reaction:4Cu O2 2Cu2O(46)we can write:( )ΔG o RT lnK RT ln p O2equilibrium Δ Ho T Δ S o(47)The line between the Cu and Cu2O domains in Fig. 10 is thus a plot of the standardGibbs energy of formation of Cu2O versus T. The temperatures indicated by thesymbols M and M are the melting points of Cu and Cu2O respectively. This line is thussimply a line taken from the well-known Ellingham diagram or ΔGo vs. T diagram for theformation of oxides. However, by drawing vertical lines at the melting points of Cu andCu2O as shown in Fig. 10, we convert the Ellingham diagram to a phase diagram.Stability domains for Cu(sol), Cu(liq), Cu2O(sol), Cu2O(liq) and CuO(sol) are shown asfunctions of T and of the imposed equilibrium pO2. The lines and triple points indicateconditions for two- and three-phase equilibria.2.5Measuring Gibbs Energy, Enthalpy and Entropy2.5.1Measuring Gibbs Energy ChangeIn general, the Gibbs energy change of a process can be determined byperforming measurements under equilibrium conditions. Consider reaction (35) forexample. Experimentally, equilibrium is first established between solid C and the gasphase and the equilibrium constant is then found by measuring the partial pressures ofCO and CO2. Eq. (36) is then used to calculate ΔGo.Another common technique of establishing equilibrium is by means of anelectrochemical cell. A galvanic cell is designed so that a reaction (the cell reaction)can occur only with the passage of an electric current through an external circuit. An18

external voltage is applied which is equal in magnitude but opposite in sign to the cellpotential, E(volts), such that no current flows. The system is then at equilibrium. Withthe passage of dz coulombs through the external circuit, Edz joules of work areperformed. Since the process occurs at equilibrium, this is the reversible non-PV work,dWrev(non-PV). Substituting Eq. (11) into Eq. (19), differentiating, and substituting Eq. (10)gives:dG V dP – S dT ΣμI dni dWrev(non-PV)(48)For a closed system at constant T and P:dGT,P,n dWrev(non-PV)(49)If the cell reaction is formulated such that the advancement of the reaction by dξ molesis associated with the passage of dz coulombs through the external circuit, then fromEq. (49):ΔG dξ - E dz(50)ΔG - lreaction,F dz/dξ 96500 coulombs mol-1 is the Faraday constant, which is the number ofcoulombs in a mole of electrons, and the negative sign follows the usualelectrochemical sign convention. Hence, by measuring the open-circuit voltage E, onecan determine ΔG of the cell reaction.2.5.2Measuring Enthalpy ChangeThe enthalpy change, ΔH, of a process may be measured directly by calorimetry.Alternatively, if ΔG is measured by an equilibration technique as in Sec. 2.5.1, then ΔHcan be determined from the measured temperature dependence of ΔG. From Eq. (48),for a process in a closed system with no non-PV work at constant pressure:(dG/dT)P,n -SSubstitution of Eq. (19) into Eq. (52) gives:19(52)

(d(G/T)/d(1/T))P,n H(53)Eqs. (52) and (53) apply to both the initial and final states of a process. Hence:(d(ΔG)/dT)P,n - ΔS(54)(d(ΔG/T)d(1/T))P,n ΔH(55)Eqs. (52) to (55) are various forms of the Gibbs-Helmholtz equation.2.5.3Measuring EntropyAs is the case with the enthalpy, ΔS o

The x-axis of this diagram is the overall molar metal ratio in the system. The phase diagram in Fig. 6 shows the equilibrium phases present when an equimolar Fe-Cr alloy is equilibrated at 925oC with a gas phase of varying O 2 and S 2 partial pressures. For systems at high pressure, P-T phase diagrams such